Difference between revisions of "Pyroelectricity"
From Online Dictionary of Crystallography
m (better translation)
|Line 1:||Line 1:|
<Font color="blue"> Pyroélectricité </Font> (''Fr''). <Font color="red"> Pyroelectrizität </Font> (''Ge''). <font color="green">Pyroelectricidad </Font> (''Sp''). <Font color="black"> Piroelettricità </Font>(''It''). <Font color="purple">
<Font color="blue"> Pyroélectricité </Font> (''Fr''). <Font color="red"> Pyroelectrizität </Font> (''Ge''). <font color="green">Pyroelectricidad </Font> (''Sp''). <Font color="black"> Piroelettricità </Font>(''It''). <Font color="purple"> </Font>(''Ja'')
Revision as of 10:31, 28 March 2015
Pyroélectricité (Fr). Pyroelectrizität (Ge). Pyroelectricidad (Sp). Piroelettricità (It). 焦電効果 (Ja)
Pyroelectricity is the property presented by certain materials that exhibit an electric polarization Pi when a temperature variation δΘ is applied uniformly:
Pi = piT δΘ
where piT is the pyroelectric coefficient at constant stress. Pyroelectric crystals actually have a spontaneous polarization, but the pyroelectric effect can only be observed during a temperature change. If the polarisation can be reversed by the application of an electric field, the crystal is ferroelectric.
If the crystal is also piezoelectric, the polarization due to an applied temperature variation is also partly due to the piezoelectric effect. The coefficient describing the pure pyroelectric effect is the pyroelectric coefficient at constant strain, piS. The two coefficients are related by:
piT = cijkldklnαjn + piS
The converse effect is the electrocaloric effect. If a pyroelectric crystal is submitted to an electric field, it will undergo a change of entropy Δσ:
Δσ = pi Ei
and will release or absorb a quantity of heat gien by Θ V Δσ where Θ is the temperature of the specimen and V its volume.
Pyroelectric point groups
The geometric crystal classes for which the piezoelectric effect is possible are determined by symmetry considerations (see Curie laws). They are the classes of which the symmetry is a subgroup of the symmetry associated with that of the electric field, A∞ ∞M:
1, 2, 3, 4, 6, m, 2mm, 3m, 4mm, 6mm
The appearance of electrostatic charges upon changes of temperature has been observed since ancient times, in particular on tourmaline. It is Sir David Brewster (1781-1788) who coined the term 'pyroelectricity' (Brewster D., 1824, Edinburgh. J. Sci., 1, 208-215, Observations on the pyroelectricity of minerals, translated into German, Poggendorf Ann. Phys., 1824, 2, 297-307, Beobachtungen über die, in den Mineralien, durch Wärme erregte Electricität).
- An introduction to crystal physics (Teaching Pamphlet of the International Union of Crystallography)
- Section 10.2 of International Tables of Crystallography, Volume A
- Section 1.1.4 and part 3 of International Tables of Crystallography, Volume D